Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

Transforming Wave Propagation in Layered Media via Instability-Induced Interfacial Wrinkling The MIT Faculty has made this article openly available. Please share how this access benefits you. Your story matters. Citation Rudykh, Stephan, and Mary C. Boyce. “Transforming Wave Propagation in Layered Media via Instability-Induced Interfacial Wrinkling.” Physical Review Letters 112, no. 3 (January 2014). © 2014 American Physical Society As Published http://dx.doi.org/10.1103/PhysRevLett.112.034301 Publisher American Physical Society Version Final published version Accessed Thu May 26 09:04:42 EDT 2016 Citable Link http://hdl.handle.net/1721.1/85082 Terms of Use Article is made available in accordance with the publisher's policy and may be subject to US copyright law. Please refer to the publisher's site for terms of use. Detailed Terms PRL 112, 034301 (2014) PHYSICAL REVIEW LETTERS week ending 24 JANUARY 2014 Transforming Wave Propagation in Layered Media via Instability-Induced Interfacial Wrinkling Stephan Rudykh* and Mary C. Boyce† Department of Mechanical Engineering, Massachusetts Institute of Technology, Cambridge 02139-4307, Massachusetts, USA (Received 13 September 2013; published 24 January 2014) The ability to control wave propagation in highly deformable layered media with elastic instability-induced wrinkling of interfacial layers is presented. The onset of a wrinkling instability in initially straight interfacial layers occurs when a critical compressive strain is achieved. Further compression beyond the critical strain leads to an increase in the wrinkle amplitude of the interfacial layer. This, in turn, gives rise to the formation of a system of periodic scatterers, which reflect and interfere with wave propagation. We demonstrate that the topology of wrinkling interfacial layers can be controlled by deformation and used to produce band gaps in wave propagation and, hence, to selectively filter frequencies. Remarkably, the mechanism of frequency filtering is effective even for composites with similar or identical densities, such as polymer-polymer composites. Since the microstructure change is reversible, the mechanism can be used for tuning and controlling wave propagation by deformation. DOI: 10.1103/PhysRevLett.112.034301 PACS numbers: 43.40.+s, 46.32.+x, 46.40.Cd Wave propagation phenomena have been investigated intensively because understanding of the phenomena is of great importance for a large variety of applications. Areas of application include nondestructive material testing, acoustic mirrors, waveguides, acoustic filters, vibration dampers, ultrasonic transducers, acoustic and optic cloaking, subwavelength imaging, and photovoltaic devices. Phononic and photonic metamaterials with periodic microstructures have attracted considerable attention [1–8]. The remarkable properties of the metamaterials originate in their microstructure, a proper choice of which may result in band gaps [1,9–17]. Soft metamaterials, due to their capability to sustain large elastic deformations, open promising opportunities of manipulating wave propagation by deformation. Deformation can influence wave propagation in two ways: first, as a material undergoes large deformation, its microstructure evolves; second, the presence of stress can influence wave propagation. Moreover, the material microstructure (geometry and constituent properties) can be tailored to give rise to elastic instabilities within the internal structure upon achieving critical strain or stress. This phenomenon can be used to trigger sudden and reversible structural pattern transformations [18,19], which can be accompanied by changes in acoustic and optical properties [20–22]. In this Letter, we specifically focus on the influence of instability-induced transformations in interfacial layers on wave propagation in finitely deformed materials. To this end, we consider layered materials with discrete interfacial layers of finite thickness with elastic modulus contrast with the surrounding matrix layers. Upon deformation, the interfacial layer will wrinkle upon reaching a critical 0031-9007=14=112(3)=034301(5) compressive strain. The wrinkle takes a sinusoidal waveform with characteristic normalized wavelength ~lcr ¼ lcr =hðiÞ can be estimated by ~lcr ¼πððð3−4νÞ=ð3ð1−νÞ2 ÞÞ ððμðiÞ Þ=ðμðmÞ ÞÞÞ1=3 , where ν is Poisson’s ratio, μ is shear modulus, and hðiÞ denotes interfacial layer thickness [19]. We use the superscripts ðÞðmÞ and ðÞðiÞ to denote the quantities associated with matrix and interfacial layers, respectively. The critical strain corresponding to the onset of instabilities is ϵcr ¼ π 2 ðlcr =hðiÞ Þ−2 . Examples of the formation of wrinkled interfacial layers are presented in Fig. 1 for composites with μðiÞ =μðmÞ ¼ 100 and interfacial layer volume fractions of cðiÞ ¼ hðiÞ =h ¼ 0.02 (red) and 0.04 (black). The post-bifurcation behavior is simulated by finite element analysis. The normalized macroscopic stress (left axis) and normalized wrinkled interface amplitude (right axis) A~ ¼ A=hðiÞ are given as a function of compressive strain [Fig. 1(c)] . The normalized mean stress is defined via σ~ ¼ σ̄ 11 =μ̄, where μ̄ ¼ cðmÞ μðmÞ þ cðiÞ μðiÞ . The dashed curve corresponds to the stress-strain relation for the composite if wrinkling were not to occur. When the compressive deformation is applied, a bifurcation is seen in the stress-strain curve upon reaching the critical strain, which triggers the instability. At this point, a sudden change in microstructure occurs and the wrinkled interfacial layers become visible with the amplitude increasing rapidly with further deformation. Compressive deformation leads to initiation and rapid growth of the amplitude of the wrinkled interface, creating a system of periodic scatterers, which reflect and interfere with propagation of elastic waves. This phenomenon allows control of wave propagation and filtering of particular bands of frequencies by application of deformation. 034301-1 © 2014 American Physical Society PRL 112, 034301 (2014) week ending 24 JANUARY 2014 PHYSICAL REVIEW LETTERS ϕ FIG. 2 (color online). Schematics of wave propagation direction with respect to interfacial layers. FIG. 1 (color online). Schematics of undeformed and deformed periodic multilayered structures with interfacial phase volume fractions (a) cðiÞ ¼ 0.02 and (b) 0.04. (c) Dependence of stress vs strain and wrinkle amplitude vs strain. The stress-strain results are given by the continuous black (cðiÞ ¼ 0.04) and red curves (cðiÞ ¼ 0.02); the dashed curve is the solution for flat layers, assuming no wrinkling. The dotted curves represent the evolution of the normalized wrinkle amplitude (right axis). The stiffness ratio of the phases is μðiÞ =μðmÞ ¼ 100. Here, we analyze the propagation of elastic waves in finitely deformed periodic materials. To this end, we consider incremental small-amplitude motions superimposed on a finitely deformed state [20]. Differently from a plane wave, a wave propagating in a periodic structure is the superposition of plane waves, which can be described by the Bloch function [1,23]. Consequently, the smallamplitude motions are implemented in terms of Bloch waves ui ðx; tÞ ¼ Ui ðx; tÞ expðik · xÞ, where ui is the displacement, k is the Bloch vector and Ui is a periodic function subjected to the periodicity condition U i ðx; tÞ ¼ Ui ðx þ a; tÞ with a being a lattice translation vector [12,20,23]. To perform this analysis, we use the finite element method, which allows us (i) to obtain the solution for the deformed periodic composite after the bifurcation, and (ii) then superimpose the Bloch-Floquet periodicity condition on the deformed state and solve the eigenvalue problem associated with the wave equations. For completeness, the numerical solution was verified against exact analytical solutions for finitely deformed infinite homogeneous and layered materials, and excellent agreement was found. We define the direction of wave propagation via angle φ as shown in Fig. 2. The influence of interface wrinkling on wave propagation is shown in Fig. 3 which compares the dispersion diagrams for (a) the undeformed state, where the applied strain ϵ ¼ 0, to (b) those at the onset of wrinkling formation ϵ ≃ ϵcr , and to (c) those for a developed wrinkled state ϵ > ϵcr . Figure 3 shows examples of dispersion diagrams for various composites with different stiffness ratios rμ ¼ μðiÞ =μðmÞ : different density contrast ratios rρ ¼ ρðiÞ =ρðmÞ , and different interfacial layer volume fractions of cðiÞ to allow comparison pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃof these effects. The normalized frequency ω~ ¼ ωh ρðmÞ =μ̄ is reported. The dispersion diagram of the undeformed structure appears in the top row. The composites present in columns (1)–(3) and (4) exhibit elastic instabilities at different levels of critical strain, in particular, at ϵcr ¼ 0.040 08 and ϵcr ¼ 0.0086, respectively. Consequently, we present the dispersion diagrams for these cases at different strain levels (middle rows), namely at ϵ ¼ 0.04 for composites in columns (1)–(3) and ϵ ¼ 0.01 for column (4). Finally, we show the dispersion diagrams for a developed wrinkled state in the bottom row for strains of ϵ ¼ 0.048 for composites in columns (1)–(3), and ϵ ¼ 0.017 for column (4). For composites present in columns (1) and (2), the normalized amplitudes of the wrinkles are A~ ¼ 0.2687 and 0.5075 at ϵ ¼ 0.04 and 0.048, respectively. The corresponding amplitudes for the composite (3) are 0.271 and 0.524, respectively. For the composite (4), the amplitudes of the wrinkles are A~ ¼ 0.522 and 1.058 at ϵ ¼ 0.01 and 0.017, respectively. The dispersion diagrams show different branches of wave propagation including transverse and longitudinal waves. In our analysis, we specifically focus on identifying complete band gaps, when both, longitudinal and transverse waves, cannot propagate. The undeformed composite does not filter waves in a direction along the interface at any frequency; however, the deformed composites with wrinkled interfaces exhibit clear band gaps [see columns (1), (2), and (4) in line (b)]. The frequency range of the band gaps is denoted by the grey filled area in Fig. 3. Note that one-dimensional phononic crystals with flat layers can never prevent wave propagation parallel to the layers [24]. In contrast, the wrinkled interfaces introduce variations of the mechanical properties in the direction of wave propagation, and, consequently, secondary waves are generated. The waves interfere with each other such that for some combination of the material properties, 034301-2 PRL 112, 034301 (2014) PHYSICAL REVIEW LETTERS week ending 24 JANUARY 2014 (1) (2) (3) (4) c(i) = 0.04, rµ =100, rρ = 5 c(i) = 0.04, rµ =100, rρ = 1 c(i) = 0.02, rµ =100, rρ = 5 c(i) = 0.04, rµ =1000, rρ = 5 (a) ε=0 ε= 0 ε = 0.01 (b) ε = 0.04 (c) ε = 0.017 ε = 0.048 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ FIG. 3. Dispersion diagrams showing normalized frequency response ω~ ¼ ωh ρðmÞ =μ̄ vs wave number for four composites: cðiÞ ¼ 0.04, rμ ¼ μðiÞ =μðmÞ ¼ 100 and rρ ¼ ρðiÞ =ρðmÞ ¼ 5 [column (1)] and rρ ¼ 1 (column 2); cðiÞ ¼ 0.02, rμ ¼ 100 and rρ ¼ 5 [column (3)]; cðiÞ ¼ 0.04, rμ ¼ 1000 and rρ ¼ 5 [column (4)]. The top row is for undeformed states. The middle is for ϵ ¼ 0.04 [columns (1)-(3)] and for ϵ ¼ 0.01 [column (4)]. The bottom row is for ϵ ¼ 0.048 [columns (1)-(3)] and for ϵ ¼ 0.017 [column (4)]. The waves propagate in an initial direction along the interface (φ ¼ π=2). geometries, wave frequencies, and amplitudes, the reflectance is such that the waves will not propagate. This situation corresponds to band gaps of forbidden frequencies as reported in Fig. 3. We observe no band gaps for the composite with low volume fractions of the interfacial layers [column (3)], even when the wrinkles are well developed. Remarkably, we find that composites with identical densities [column (2)] produce band gaps when the wrinkling interfaces are induced. Finally, for the composites with a higher contrast in the stiffness of the phases, namely rμ ¼ 1000 [column (4)], we observe that the band gap appeared after wrinkle formation, but the band gap narrowed with further deformation, whereas the band gap broadened for the case with lower stiffness ratio. The development of band gaps with deformation is shown in Fig. 4 for composites with cðiÞ ¼ 0.04 and rμ ¼ 100 with density ratios rρ ¼ 1 (left column) and 5 (right column). Figure 4 shows the evolution of the prohibited frequency ranges as a function of strain for different directions of wave propagation φ ¼ π=2, 0, and π=4 (from top to bottom). For waves traveling along the layers, φ ¼ π=2, the band gap that appears upon wrinkling initiation shifts to a lower frequency band. The band gap widens due to the evolution in scattering as the wrinkle waveform amplitude and wavelength evolve. There is a change in the band-gap evolution at ϵ ≃ 0.045, when the band gap starts shifting toward higher frequencies. For waves traveling in the direction perpendicular to the layers (φ ¼ 0) and rρ ¼ 5, there are two initial band gaps. The first band gap, at higher frequencies, gradually widens with increasing strain. The second band gap, of lower frequencies, rapidly narrows with the deformation until it closes at ϵ ≃ 0.005. This is followed by immediate reopening of the band gap and further widening until ϵ ≃ 0.0075, after which the band-gap width remains constant. For the waves traveling at φ ¼ 0 in the composite of rρ ¼ 1, one band gap is observed. The band gap opens at ϵ ≃ 0.018 and then rapidly widens until ϵ ¼ 0.021, after which it continues to widen, although slowly. At ϵ ≃ 0.04, the band gap starts to narrow due to the decrease of the upper boundary, while the lower boundary remains constant. For oblique waves traveling at φ ¼ π=4, the opening and evolution of band gaps are similar to that observed for the case of φ ¼ π=2. We showed that band gaps can be created in composites with identical densities of the phases when the interfaces take on a wavy topology. The case when both phases have similar densities is of great interest due to the potential for manufacturing light-weight polymer acoustic metamaterials. To highlight the role of the density contrast rρ , we present the band gaps as functions of density contrast rρ in Fig. 5. The examples are given for composites with cðiÞ ¼ 0.04 and initial stiffness ratios rμ ¼ 100 (left column) and 1000 (right column). We consider deformation at ϵ ¼ 0.048 (left) and 0.017 (right), where the wrinkled interfaces are developed. The prohibited frequency 034301-3 PRL 112, 034301 (2014) PHYSICAL REVIEW LETTERS week ending 24 JANUARY 2014 FIG. 4. The prohibited frequency domains and the amplitude of the wrinkled interface as functions of applied strain. The initial stiffness ratio is rμ ¼ 100, and density contrast ratio is rρ ¼ 1 (left) and 5 (right). The wave propagation directions are φ ¼ π=2, φ ¼ 0, and φ ¼ π=4 (from top to bottom). domains are given for different directions of wave propagation φ ¼ π=2, φ ¼ 0, and φ ¼ π=4 (from top to bottom). For waves traveling at φ ¼ π=2 in the composite of rμ ¼ 100, a band gap appears at rρ ¼ 1. The band gap shifts toward lower frequencies with an increase of rρ . For the normal wave propagation (φ ¼ 0), we observe a rather narrow band gap at rρ ¼ 1. However, the band gap widens significantly with an increase of rρ . Additionally, two new band gaps opens at rρ ≃ 3.6 and 6, respectively. For oblique waves traveling at φ ¼ π=4, the maximum width of the band gap is reported at rρ ¼ 1. The band gaps gradually narrow with an increase of rρ due to both decreasing of the upper boundary and increasing of the lower boundary. The band gap closes at rρ ≃ 10. Composites with the higher stiffness ratio (rμ ¼ 1000) exhibit a narrow band gap for wave propagation along the layers (φ ¼ π=2). For propagation normal to the interface (φ ¼ 0), the composite possesses a band gap that broadens with increasing density contrast as well as the emergence of a second band gap when the density ratio exceeds 7. For oblique propagation (φ ¼ π=4), this composite does not have a band gap. We revealed transformation of wave propagation via instability-induced interfacial wrinkling in composites with interfacial layers. We demonstrated that the formation of the wrinkling interfaces can be used to create band gaps and filter undesirable frequencies. These frequency bands are highly tunable by the material choice and the thickness of layers and the distance between the layers. Since the microstructure change is reversible, the phenomenon is also tunable and reversible depending on the applied stress or deformation. Consequently, we present a novel ability to FIG. 5. The prohibited frequency domain as a function of density ratio rρ for rμ ¼ 100 at post-bifurcated state of ϵ ¼ 0.045 (left) and for rμ ¼ 1000 at ϵ ¼ 0.017 (right) considering interfacial volume fraction of cðiÞ ¼ 0.04. The wave propagation directions are φ ¼ π=2, φ ¼ 0, and φ ¼ π=4 (from top to bottom). actively control wave propagation in layered materials. Moreover, this ability applies to material layers with similar or even identical densities of the phases. Besides the propagation of elastic waves in media with instability-induced interfacial wrinkling, the concept of transforming the wave propagation extends further and can be applied to development of switchable photonic crystals. These optical structures are widely present in nature. However, they are still a challenge to manufacture and are even more challenging to actively control. The study described in this Letter opens up a new prospect for advancing the technology for tunable photonic crystals. The similarities in the phenomena of elastic and electromagnetic (in particular, the optical case) wave propagation, point towards the possibility of extending the idea to switchable photonic crystals. Design of the tunable photonic structures will require additional analyses due to the differences in the phenomena; in particular, elastic waves propagate in longitudinal and transverse modes (these are not pure modes, in general), whereas the polarization of the electromagnetic waves is transverse [25]. Layered materials with varying mechanical and optical phase properties can be manufactured even with ultrathin and subwavelength thicknesses of the layers [26]. Mechanical loadings can be used to induce and control the wrinkling patterns, which may give 034301-4 PRL 112, 034301 (2014) PHYSICAL REVIEW LETTERS rise to a variety of optical effects; for example, silvery iridescence around the eyes of squid (L. pealeii) due to the wrinkling pattern of thin layers (80–130 nm [27]) may be mimicked. Moreover, the effect can be further actively controlled by varying the stress or deformation and, as a result, changing the amplitude of the wrinkling interfaces. This research was supported by the U.S. Army Research Office through the MIT Institute for Soldier Nanotechnologies under Contract No. W911NF13-D-0001. * Corresponding author. rudykh@mit.edu † Present address: School of Engineering and Applied Science, Columbia University, New York, New York 10025, USA. [1] M. S. Kushwaha, P. Halevi, L. Dobrzynski, and B. DjafariRouhani, Phys. Rev. Lett. 71, 2022 (1993). [2] T. Gorishnyy, C. Ullal, M. Maldovan, G. Fytas, and E. Thomas, Phys. Rev. Lett. 94, 115501 (2005). [3] A. Akimov, Y. Tanaka, A. Pevtsov, S. Kaplan, V. Golubev, S. Tamura, D. Yakovlev, and M. Bayer, Phys. Rev. Lett. 101, 033902 (2008). [4] X.-F. Li, X. Ni, L. Feng, M.-H. Lu, C. He, and Y.-F. Chen, Phys. Rev. Lett. 106, 084301 (2011). [5] S. Zhang, C. Xia, and N. Fang, Phys. Rev. Lett. 106, 024301 (2011). [6] C. Genet and T. Ebbesen, Nature (London) 445, 39 (2007). [7] S. Zhang, D. Genov, Y. Wang, M. Liu, and X. Zhang, Phys. Rev. Lett. 101, 047401 (2008). [8] G. Weick, C. Woollacott, W. Barnes, O. Hess, and E. Mariani, Phys. Rev. Lett. 110, 106801 (2013). [9] M. S. Kushwaha, P. Halevi, G. MartÃnez, L. Dobrzynski, and B. Djafari-Rouhani, Phys. Rev. B 49, 2313 (1994). week ending 24 JANUARY 2014 [10] A. H. Nayfeh, Wave Propagation in Layered Anisotropic Media: with Applications to Composites (Elsevier Science, New York, 1995). [11] M. Aberg and P. Gudmundson, J. Acoust. Soc. Am. 102, 2007 (1997). [12] Y. Tanaka, Y. Tomoyasu, and S.-I. Tamura, Phys. Rev. B 62, 7387 (2000). [13] J. O. Vasseur, P. A. Deymier, A. Khelif, P. Lambin, B. Djafari-Rouhani, A. Akjouj, L. Dobrzynski, N. Fettouhi, and J. Zemmouri, Phys. Rev. E 65, 056608/1 (2002). [14] O. Sigmund and J. Jensen, Phil. Trans. R. Soc. A 361, 1001 (2003). [15] H. Zhao, Y. Liu, G. Wang, J. Wen, D. Yu, X. Han, and X. Wen, Phys. Rev. B 72, 012301 (2005). [16] M. Gei, Eur. J. Mech. A. Solids 27, 328 (2008). [17] L. Hu, L. Liu, and K. Bhattacharya, J. Elast. 107, 65 (2012). [18] T. Mullin, S. Deschanel, K. Bertoldi, and M. C. Boyce, Phys. Rev. Lett. 99, 084301 (2007). [19] Y. Li, N. Kaynia, S. Rudykh, and M. C. Boyce, Adv. Eng. Mater. 15, 921 (2013). [20] K. Bertoldi and M. C. Boyce, Phys. Rev. B 78, 184107 (2008). [21] J.-H. Jang, C. Y. Koh, K. Bertoldi, M. C. Boyce, and E. L. Thomas, Nano Lett. 9, 2113 (2009). [22] L. Wang and K. Bertoldi, Int. J. Solids Struct. 49, 2881 (2012). [23] C. Kittel, Introduction to Solid State Physics (Wiley, New York, 2004), 8th ed.. [24] M. Maldovan and E. L. Thomas, Periodic Materials and Interference Lithography: for Photonics, Phononics and Mechanics (Wiley-VCH, Weinheim, 2009). [25] E. G. Henneke and R. E. Green, J. Acoust. Soc. Am. 45, 1367 (1969). [26] M. Kats, S. Byrnes, R. Blanchard, M. Kolle, P. Genevet, J. Aizenberg, and F. Capasso, Appl. Phys. Lett. 103, 101104 (2013). [27] L. Mathger, E. Denton, N. Marshall, and R. Hanlon, J. R. Soc. Interface 6, S149 (2009). 034301-5

Similar